230 



Tables 229-230. 

 TABLE 229. — Speclllc Heat of Various Solids.* 



Solid. 



Alloys : 



Bell metal 



Brass, red 



" yellow 



8o Cu-j-20 Sn 



88.7 Cu+i 1.3 Al 



German silver 



Lipowitz alloy: 24.97 Pb + 10.13 Cd + 50.66 Bi 

 +14.24 Sn . . . . 



Rose's alloy : 27.5 Pb+48.9 Bi+23.6 Sn 



Wood's alloy : 25.85 Pb + 6.99 Cd + 52.43 Bi + 



1473 Sn 



" " (fluid) 



Miscellaneous alloys : 

 17.5 Sb+29.g Bi4-i8.7 Zn+33.9 Sn . . . 



37.1 Sb+62.9 Pb 



39.9 Pb-j-6o.i Bi 



" (fluid) 



63.7 Pb+36.3 Sn 



46.7 Pb+53.3 Sn 



63.8 Bi+36.2 Sn 



46.9 Bi+53.1 Sn 



Gas coal 



Glass, normal thermometer 16°^ 



" French hard thermometer .... 



crown 

 flint . 



Ice 



India rubber (Para) 

 Paraffin 



" fluid . 

 Vulcanite 



Temperature 



15-98 

 O 



o 



14-98 



20-100 



O-IOO 



s-50 



100-150 



—77-20 



20-89 



5-50 

 100-150 



20-99 

 10-98 



16-99 

 144-358 



12-99 

 10-99 

 20-99 

 20-99 

 20-1040 

 19-100 



10-50 



10-50 



-188 252 



—78 188 



_i8 78 



.'-lOO 



—20- +3 



— 19-4-20 



0-20 



35-40 

 60-63 



Specific Heat. 



.08831 

 .0862 

 .10432 

 .09464 



•0345 

 .0426 



•0356 

 .0552 



•0352 

 .0426 



.05657 

 .03880 

 .03165 

 .03500 

 .04073 

 .04507 

 .04001 

 .04504 

 •3145 



.161 



.117 



.146 



.285 



•463 



.481 



.3768 



•5251 



•6939 

 .622 

 .712 

 •3312 



Authority, t 



R 



L 



(i 



R 

 Ln 

 T 



M 



(( 



S 



u 



M 

 R 



it 



P 



(( 



R 



W 



Z 



H M 



D 



G-T 

 R W 



B 



A M 



TABLE 230. — Specific Heat of Various Liquids.* 



• These specific heat tables are compiled partly from more extended tables in Landolt-Bornstein-Meyerhoffer's Tables, 

 t For references see Table 230, page 231. 

 Smithsonian Tables. 



